Visible light-induced photocatalytic and antibacterial adhesion properties of superhydrophilic TiO2 nanoparticles

Bacterial infections triggered by patient or healthcare worker contact with surfaces are a major cause of medically acquired infections. By controlling the kinetics of tetrabutyl titanate hydrolysis and condensation during the sol–gel process, it is possible to regulate the content of Ti3+ and oxygen vacancies (OVs) in TiO2, and adjust the associated visible light-induced photocatalytic performance and anti-bacterial adhesion properties. The results have shown that the Ti3+ content in TiO2 was 9.87% at the calcination temperature of the reaction system was 300 °C and pH was 1.0, corresponding to optimal photocatalytic and hydrophilic properties. The formation of a hydrated layer on the superhydrophilic surface provided resistance to bacterial adhesion, preventing cross-contamination on high-touch surfaces. The excellent photocatalytic self-cleaning performance and anti-bacterial adhesion properties can be attributed to synergistic effects associated with the high specific surface area of TiO2 nanoparticles, the mesoporous structure, and the presence of Ti3+ and OVs. The formation of superhydrophilic self-cleaning surfaces under visible light can serve as the basis for the development of a new class of anti-bacterial adhesion materials.

Modified TiO 2 exhibits high efficacy in inactivating a wide range of bacteria and viruses under visible light and has been widely used in dental, orthopedic, and bone implants to prevent bacterial infections [22][23][24][25] .In addition, superhydrophilic TiO 2 with a visible light response has been applied as a coating for surfaces such as automotive glass, construction materials, and medical devices due to its enhanced self-cleaning and antifouling properties 13 .A superhydrophilic TiO 2 surface provides resistance to bacterial adhesion, thereby effectively inhibiting the formation of biofilms.Hu et al. 26 have proposed that the anti-bacterial adhesion mechanism of superhydrophilic materials can be attributed to the creation of a surface hydrated layer that exhibits repulsive and spatial site-barrier effects.This hydrated layer acts as a barrier, preventing bacteria from penetrating, contacting, and adhering to the material 27 .There have been few studies that address utilization of superhydrophilic properties to inhibit biofilm formation, and most studies have focused on superhydrophobic surfaces [28][29][30] .Superhydrophilic surfaces are more conducive than superhydrophobic surfaces to antimicrobial release 31 .Consequently, the application of self-cleaning nano-TiO 2 , which exhibits superhydrophilicity and resistance to bacterial adhesion under visible light warrants further investigation.
In this study, a superhydrophilic, strongly visible-light-responsive Ti 3+ and OVs-doped TiO 2 with excellent photocatalytic activity and resistance to bacterial adhesion has been developed.The crystal conformation, surface properties, and defect structure of anatase TiO 2 nanoparticles were modulated by controlling the pH and calcination temperature.We have evaluated the ability of TiO 2 , synthesized at different pH and calcination temperatures, to degrade methyl orange (MO) under simulated sunlight (full-spectrum) and visible light radiation exposure.The mechanism of MO photocatalytic oxidation has been examined using free radical detection.In addition, we have investigated the hydrophilic properties of different TiO 2 under natural light.The ability of the hydrophilic films to resist adhesion of E. coli was quantitatively investigated using the plate coating method.The defect structure of TiO 2 can be controlled using a simple method to broaden its absorption spectrum, resulting in improved photocatalytic activity and antibacterial adhesion properties under visible light.The findings of this study provide theoretical support for the future application of TiO 2 in the medical field to prevent bacterial infections caused by medical personnel coming into contact with infected surfaces.

Preparation of anatase TiO 2
Titania (TiO 2 ) was synthesized using a low temperature sol-gel method, as shown in Fig. 1.Tetrabutyl titanate (TBOT) was slowly added to anhydrous ethanol to form a TBOT master-batch with a molar concentration of 0.59 M. A 24 mL sample of the TBOT master-batch was measured and labeled "solution A".A 2 mL volume of diluted acetic acid solution (2% by mass) was added to a beaker containing 35 mL of anhydrous ethanol with hydrochloric acid (HCl) as a catalyst, and the pH was adjusted to give solution B. At a H + /Ti molar ratio of 0, 0.001, 0.2 and 0.5, the corresponding pH was 0.6, 1.0, 1.9 and 4.7, respectively.A peristaltic pump was used to deliver solution A dropwise into solution B at a rate of 3 mL/min.The mixture was then agitated in a water bath at 25 °C for 3 h to produce a sol, and following a 20 h aging period, a gel was formed.The resultant samples were dried at 120 °C for 6 h, and treated in air at 300, 400, 500, 600, and 700 °C for 2 h using a heating rate of 4 °C/min.www.nature.com/scientificreports/Finally, the calcined samples were ground in agate to obtain TiO 2 powder.The samples are denoted as TN-X-Y, where X represents the pH and Y represents the calcination temperature.Titania films were also prepared.Microscope coverslips and slides were used as substrates for the TiO 2 films, which were ultrasonically cleaned sequentially with acetone, anhydrous ethanol, and deionised water before use to remove organic and inorganic contaminants.The surfaces were then dried and made ready for use.Slides were utilized for assessing anti-bacterial adhesion whereas coverslip substrates were employed for contact angle testing.The TiO 2 powder was dissolved in anhydrous ethanol and subjected to ultrasonication for 30 min to produce a suspension with a concentration of 13 g/L.The application of the films onto the glass substrate was performed using a constant-temperature impregnation lift coater (Shanghai Sanyan Technology, SYDC-200H) with a descending speed of 3 mm/s, lifting speed of 1 mm/s, impregnation time of 30 s, retention time of 120 s, and six coatings.

Morphological and chemical characteristics
Surface elemental analysis was conducted using an X-ray photoelectron spectrometer (XPS, Thermo Fisher Scientific, Thermo Scientific ESCALAB Xi +).Specific surface area and pore size analyses were performed using a specific surface area tester (BET, Bayside Instrument Technology (Beijing), BSD-660S A6).Oxygen vacancy and photogenerated radical testing were carried out using electron paramagnetic resonance (EPR, Germany, Bruker EMX PLUS).The light absorption spectra of TiO 2 in the wavelength range of 200-800 nm were measured using a UV-Vis diffuse reflectance spectrometer (UV-Vis-DRS, Shimadzu, UV-2700i).The physical phase composition of the materials was analyzed using an X-ray diffractometer (XRD, Shimadzu, XRD-7000S) over a 2θ scanning range from 20° to 80° and a scanning speed of 2°/min.The crystal size of the anatase TiO 2 (101) crystalline faces was calculated using the Scherrer Equation 32 .The infrared spectra (IR) of the samples (prepared as KBr tablets) were obtained on a Fourier transform infrared spectrometer (IR Prestige-21, SHMADZU).Thermogravimetric analysis (TGA) of the samples was performed using a TA instrument (TGA/DSC1/1600LF, Mettler Toledo).

Hydrophilicity test
The static water contact angle (WCA) of the TiO 2 films was determined using a video contact angle tester (Drop-MeterTM A-200, Ningbo Haishu Maishu Inspection Technology Co., Ltd).A 2.0 μL droplet was placed on the TiO 2 film using a syringe.The droplet shape was then captured using a CCD camera, and the static contact angle of water subsequently calculated.The water droplets were placed at four different locations for each sample, and the average contact angle value was determined.

Evaluation of photocatalytic activity
A xenon lamp was used as a simulated sunlight source (full-spectrum), whereas visible light with a wavelength of 420-800 nm was employed to degrade methyl orange (MO) at a photocurrent of 15 mA.The degradation of MO by TiO 2 samples was assessed using an ultraviolet-visible spectrophotometer (UV-Vis).The experiment was conducted at room temperature by adding 50 mg anatase TiO 2 (0.5 g/L) to a 100 mL solution of MO with an initial concentration of 5 mg/L.The mixture of photocatalyst and MO was allowed to reach adsorption-desorption equilibrium by incubating in the dark for 60 min.During the photoreaction phase, the mixed solutions were exposed to simulated sunlight for 1 h.Samples were collected at 10-min intervals, and the concentration of MO remaining was determined by UV-Vis analysis (at 464 nm).In addition, the reaction was conducted under visible light irradiation for 2 h.Samples were taken at 20-min intervals to monitor the residual concentration of MO using the same method.

Anti-bacterial adhesion assay
The anti-adhesion experiment was performed using the Gram-negative strain E. coli ATCC 25,922.A 3 mL sample of LB liquid medium was added to two 12 mL bacterial culture tubes.Single colonies were selected from the E. coli solid medium and transferred to the liquid medium; the second liquid medium served as a blank.The samples were placed in a constant temperature shaker (37 °C, 200 rpm) and incubated for 15 h.The bacterial solution was then diluted to 10 6 CFU/mL using a saline solution (0.85% NaCl).A 304 μL sample of the bacterial solution was uniformly added to the sample surface.The dimensions of the glass matrix were 2.5 cm × 7.6 cm.Sterilized tweezers were used to pick up the sterilized cover film and individually cover the samples, ensuring that it was spread flat so that the bacteria touched the samples.The surfaces were evenly coated with bacteria, ensuring that they did not extend beyond the edges of the covering film.The surfaces were then incubated at 37 °C for 6 h for bacterial adhesion.After this period, the samples were carefully picked up using sterile forceps and washed three times with saline to remove any bacteria that did not fully adhere.The washed samples were transferred to new petri dishes, and 20 mL saline solution was added.Ultrasound was applied for 15 min to completely dislodge the adhering bacteria.Serial tenfold dilutions of the bacterial solution utilized sterile PBS solution.A 100 μL sample of the diluted bacterial suspension was taken from the tubes, evenly spread onto the MHA plate, and incubated for 18 h at 37 °C.The plate was removed, and photographed, recording the number of colonies.
www.nature.com/scientificreports/A conversion of TiO 2 from anatase to rutile was observed in the case of TN-0.6-700.At a high concentration of HCl, the surface energy of the TiO 2 crystals increases, which facilitates conversion of anatase to rutile 33 .The crystallinity of TiO 2 was reduced at a calcination temperature of 300 °C and deteriorated with increasing pH (Fig. 2).The findings suggest that a decrease in pH is accompanied by larger crystalline grains.A positive correlation between calcination temperature and TiO 2 grain size, as determined by the Scherrer equation, is shown in Fig. S2.It should be noted that sample TN-4.7, which did not undergo hydrochloric acid treatment, exhibited the largest grain size.A slight decrease in grain size was observed with decreasing pH after the addition of hydrochloric acid.The grain sizes of TN-0.6-300,TN-1.0-300,TN-1.9-300, and TN-4.7-300 were 8.7, 9.9, 11.4, and 16.1 nm, respectively.The observed dependence of grain size on pH may be attributed to the repulsive effect of H + with respect to positively charged Ti ions when HCl is added, resulting in the formation of TiO 2 with a smaller grain size 34 .

TEM analysis
The surface morphology, grain size, and exposed crystal surface of TN-0.6-300,TN-1.0-300,TN-1.9-300, and TN-4.7-300 were analyzed by transmission electron microscopy (TEM) and high-resolution transmission electron microscopy (HRTEM), as shown in Fig. 3.The TEM images offer evidence of sample spherical morphology with well-defined grain boundaries.The results indicate that pH does not significantly affect the morphology of TiO 2 .The HRTEM images reveal that the primary lattice spacing for TiO 2 prepared at different pH is ca.0.35 nm.This spacing corresponds to the (101) anatase plane, which is known for exhibiting superior thermal stability relative to other facets of anatase 35 .It should be noted that the HRTEM analysis of TN-0.6-300 has revealed the presence of the (101) plane associated with the exposed crystal surface, and the (200) plane with a lattice spacing of ca.0.19 nm (Fig. 3b).In contrast, TN-1.0-300 exhibits the (001) plane with a lattice spacing of ca.0.24 nm, as illustrated in Fig. 3e.The histograms illustrating particle size distributions have established average particle sizes for TN-0.6-300,TN-1.0-300,TN-1.9-300, and TN-4.7-300 of 10.1, 9.9, 11.2, and 17.0 nm, respectively.The observed grain sizes at the four pH values are consistent with the grain sizes calculated using the Scherrer equation.

XPS and EPR analysis
XPS measurements were employed to analyze the surface chemical composition and valence states of the samples.The high-resolution O1s and Ti2p spectra for TN-0.6-300,TN-1.0-300,TN-1.9-300, and TN-4.7-300 are presented in Fig. 4a-h.It can be seen that the O1s spectrum presents three peaks with binding energies of 529.6, 531.3, and 532.4 eV.These peaks are associated with Ti-O-Ti bonds, and surface adsorbed -OH, and OVs that are in close proximity to Ti 3+ , respectively, which provide evidence for the presence of Ti 3+36-38 .The Ti 2p spectrum exhibits four characteristic peaks at binding energies of 458.65, 464.42, 457.78, and 462.21 eV.These peaks can be attributed to the 2p 3/2 and 2p 1/2 orbitals of Ti 4+ and Ti 3+ ions, respectively, confirming the presence of Ti 3+ .The intensity of Ti 3+ followed the order, TN-1.9-300 > TN-1.0-300 > TN-0.6-300 > TN-4.7-300, with values of 10.69%, 9.87%, 9.32%, and 8.86%, respectively.It should be noted that the -OH and OVs peaks for TN-1.9-300 are shifted by 0.76 and 0.68 eV to higher binding energies, respectively.This shift can be attributed to a lattice distortion caused by a strong interaction between OVs and Ti 4+ ions.High concentrations of OVs, which maintain a positive charge, serve to repel Ti towards neighboring OVs.This repulsion reduces the Ti-O bond length and increases the binding energy of O1s 39 .
The presence of OVs is further confirmed by the EPR analysis, shown in Fig. 5.The EPR spectra of asprepared samples show intense axially symmetry signals centered on the g = 2.004, which have been extensively reported for Ti 3+ ions in anatase crystallite 40,41 .Moreover, the variation in the EPR signal associated with OVs is www.nature.com/scientificreports/consistent with the order of Ti 3+ content determined by XPS.This means that the intensity of OVs decreased as the pH decreased in the presence of HCl as a catalyst.At low pH, the TBOT hydrolysis rate is inhibited, resulting in incomplete hydrolysis, with a consequent generation of OVs 42 .Further investigation is required to elucidate the underlying mechanism whereby pH influences the production of OVs.It is obvious that the signal intensities associated with OVs is consistent with the order of Ti 3+ content determined by XPS.The presence of OVs decreases the rate of TiO 2 photogenerated e − -h + recombination, increasing the rate of reactive oxygen species (ROS) generation, and enhances the generation of hydroxyl groups on the surface of TiO 2 , thereby contributing to photocatalytic activity 43,44 .

BET surface areas and pore distributions
The specific surface area and pore size distribution of TiO 2 samples prepared at different pH were determined from low-temperature nitrogen adsorption-desorption measurements, and the results are shown in Fig. 6.The isotherms of all the samples correspond to type IV (BDDT classification), exhibiting an obvious hysteresis loop (Type H2), indicating a mesoporous structure 45 .Both the specific surface area and pore size decreased in the order, TN-1.0-300 > TN-4.7-300 > TN-0.6-300 > TN-1.9-300.The corresponding surface areas are 91.7,87.1, 67.7, and 66.1 m 2 /g, and the associated pore sizes are 7.8, 7.7, 7.4, and 5.5 nm, respectively.The TN-1.0-300 sample exhibited a narrow pore size distribution (Fig. 6b), indicating the formation of regular pore channels in the mesoporous region.Moreover, TN-1.0-300 is characterized by a higher specific surface area and larger grain www.nature.com/scientificreports/size, which should result in enhanced photocatalytic activity.A high surface area increases the number of available active sites for the adsorption of pollutant molecules and reduces the rate of electron-hole complexation 46 .This, in turn, enhances the efficiency of photocatalytic degradation of dyes.In addition, a larger average pore size facilitates the entry of organic pollutants into the pores, thereby increasing the efficiency of dye decomposition 47 .

Optical properties
The spectral absorption range and energy band gap of TiO 2 were examined using UV-Vis DRS to identify samples that demonstrate a high level of light absorption, a narrow energy band gap, and a shift to longer wavelengths in terms of light absorption.Based on the UV-Vis absorption spectra presented in Fig. 7a and Fig. S3a, it is evident that all the samples show a significant optical absorption peak below 400 nm.This peak can be attributed to the absorption associated with the intrinsic band gap of TiO 2 .In the case of TN-1.0-300, the optical absorption edge of TiO 2 is slightly red-shifted to ca. 410 nm when the calcination temperature was increased from 400 to 700 °C.At a calcination temperature of 300 °C, TiO 2 prepared at different pH exhibited strong light absorption in the visible wavelength range from 400 to 800 nm.The dependence of the energy band gap of TiO 2 on calcination temperature is presented in Fig. S3c, where it is evident that sample synthesis at 300 °C resulted in the smallest energy band gap.The band gaps, as shown in Fig. 7b, follow the order, TN-4.7-300 > TN-0.6-300 > TN-1.0-300 > TN-1.9-300, with corresponding values of 2.58, 2.37, 2.18, and 1.94 eV, respectively, which are all lower than 3.2 eV 21 .The relationship between the energy band gap and the intensity of the EPR OVs signal indicates that a smaller energy band gap is associated with a stronger signal.This response suggests that the presence of Ti 3+ and OVs is an important factor contributing to the redshift in the optical absorption range and the decrease in the energy band gap of TiO 2

48
. In addition, the enhanced absorbance in the visible range of the samples may be related to the presence of impurities caused by incomplete decomposition of organic compound and amorphous metatitanic acid (Ti(OH) 4 ) due to low calcination temperature (Figs.S4, S5).

Photocatalytic degradation activity
The photocatalytic activity of TiO 2 , prepared under different conditions, was assessed by measuring the degradation rate of MO solutions under simulated sunlight and visible light radiation.Before subjecting the MO to radiation degradation using a xenon lamp as a light source, all the samples reached adsorption-desorption equilibrium at 700 rpm in the dark.Blank experiments established that the concentration of MO did not change in the absence of a TiO 2 catalyst.
In order to investigate the impact of calcination temperature (300-700 °C) on the photocatalytic degradation of MO, TN-1.0 was chosen as a representative system.The results, presented in Fig. S6, indicate that MO photocatalytic degradation efficiency decreased with increasing calcination temperature under both simulated sunlight (Fig. S6a) and visible light irradiation (Fig. S6b).This can be attributed to the increase in grain size at higher temperatures established by XRD analysis, where a larger particle size lowers the number of active sites 49 .It was observed that TiO 2 delivered lower photocatalytic activity under visible light at temperatures above 400 °C, but the activity at 300 °C was only slightly lower than that achieved under simulated sunlight.This can be ascribed to the lower energy band gap of TiO 2 at this temperature.The MO degradation curves under simulated sunlight for samples calcined at 300 °C with varying pH are shown in Fig. 8a.The photocatalytic activity decreased in the order, TN-1.0-300 ≥ TN-0.6-300 > TN-4.7-300 > TN-1.9-300 > P25.The associated first-order kinetic constants (k) exhibit the same trend, with values of 0.182, 0.181, 0.082, 0.015 and 0.008 min −1 , respectively.(Fig. 8b).A switch to visible light radiation resulted in an increase in reaction time from 60 to 120 min (Fig. 8c).After 120 min of visible light irradiation, MO concentration did not change over TiO 2 (P25), but the as-prepared samples exhibited good visible light activity.The trends in terms of photocatalytic activity response to pH levels were consistent with that observed for simulated solar radiation.The TN-1.0-300 catalyst delivered the highest level of MO photodegradation, followed by TN-0.6-300where the conversion was significantly lower.The variation of the rate constant (Fig. 8d) follows the same trend as observed under simulated solar radiation, with values of 0.081, 0.020, 0.010 and 0.005 min −1 for TN-1.0-300,TN-0.6-300,TN-4.7-300 and TN-1.9-300, respectively.
The enhanced photocatalytic activity associated with TN-1.0-300 under both simulated sunlight and visible light can be attributed to several factors.Firstly, the presence of Ti 3+ and OVs reduces the energy band gap of TiO 2 and elevates photocatalytic activity.The photocatalytic activity of TiO 2 is directly proportional to the content of Ti 3+ and OVs.However, an excessive Ti 3+ and OVs content in TN-1.9-300 results in the formation of an e − -h + www.nature.com/scientificreports/complex center that lowers photocatalytic activity 50 .Photogenerated radical production, as tested by EPR, has revealed that the characteristic signal peaks due to DMPO-•O 2 − and DMPO-•OH appeared in the spectra for both TN-1.0-300 and TN-0.6-300 after 20 min of radiation under visible light.Moreover, the production rates of •O 2 − and •OH in TN-1.0-300 were faster than TN-0.6-300, as shown in Fig. 9.This suggests that TN-1.0-300 exhibits a lower photogenerated e-h + complexation rate than TN-0.6-300, and generates more free radicals under the same conditions.The appearance of OVs, •O 2 − , and •OH confirms a high photocatalytic activity for TN-1.0-300.In addition, TiO 2 prepared under these conditions is characterized by a smaller grain size and higher crystallinity.A decrease in grain size enhances the diffusion rate of photogenerated carriers from the interior of TiO 2 to the surface, resulting in an increased photocatalytic efficiency 51 .TN-1.0-300 also exhibits the largest specific surface area and pore size, which facilitates light absorption due to the greater number of active sites 52 .Furthermore, the presence of exposed (001) crystalline planes, established by TEM analysis, contributes to the improved photocatalytic performance of TN-1.0-300.Photogenerated electrons are mainly enriched in the (101) plane, whereas photogenerated holes predominate in the (001) plane facets.The occurrence of both (001) and (101) crystalline planes in a certain ratio forms crystalline heterojunctions, which serve to reduce the recombination of electrons and holes 53 .

Hydrophilic properties
The hydrophilicity of TiO 2 prepared using different process conditions was assessed by observing the water contact angle (WCA) of droplets on a film under natural light conditions, as shown in Fig. 10a.It can be seen that the WCA ranges from 4.6° to 17.4°, indicating that the TiO 2 samples exhibit excellent hydrophilic properties, and can even reach the superhydrophilic level.The WCA increased with increasing calcination temperature for different pH values.Given the relationship of grain size with temperature, it can be inferred that changes in grain size are positively correlated with the contact angle.This observation offers new possibilities for enhancing material hydrophilicity by regulating morphology.However, TN-4.7-300 which has the largest grain size was characterized by the smallest WCA.This indicates that the factors affecting the hydrophilicity of TiO 2 are not singular 54 .
The contact angle of TiO 2 , prepared at various pH values and calcined at 300 °C, has been measured and the results are presented in Fig. 10b-e.Sample TN-1.0-300 exhibited the largest WCA, followed by TN-1.9-300,TN-0.6-300, and the smallest WCA was associated with TN-4.7-300; the values are 7.8, 6.7, 6.4, and 4.7°, respectively.Based on the findings of Yang et al. 55 , who controlled the synthesis of hydrophilic or hydrophobic membranes by manipulating the hydrolysis-condensation rate of silica precursors, it can be inferred that the variation in TiO 2 WCA at different pH may be attributed to the extent of TBOT hydrolysis caused by the addition of varying amounts of HCl.An increased HCl addition, with a consequent lower pH, inhibited hydrolysis to a greater extent.However, TBOT can be synthesized in the form of a titanium sol that consists of hydrophilic (-OH) and hydrophobic (-CH 3 ) groups due to complete and incomplete hydrolysis, respectively.At a pH of 4.7, the TBOT precursor underwent complete hydrolysis without the addition of HCl as a hydrolysis inhibitor, leading to the optimal hydrophilic characteristics observed in TN-4.7-300.Moreover, TN-1.9-300 and TN-1.0-300 exhibited hydrophilic properties that are consistent with this reasoning.However, this is not the case for TN-0.6-300, which exhibits high hydrophilicity due to the high hydroxyl content, as determined by XPS analysis 56 .The results have established that TiO 2 exhibits the best hydrophilic properties at a calcination temperature of 300 °C.

Inhibition of bacterial adhesion
The adhesion E. coli to TiO 2 films is illustrated in Fig. 11a-d for bacteria diluted by a factor of 1 × 10 2 before incubation, and in Fig. 11e-h for bacteria diluted by a factor of 1 × 10 3 .Following bacteria adherence to the surface of   www.nature.com/scientificreports/different films, and subsequent dilution and incubation using the plate spread method, the number of bacteria colonies on the films decreased in the order, TN-1.0-300 > TN-1.9-300 > TN-0.6-300 > TN-4.7-300.The corresponding surface bacterial adherence was 4.26 × 10 6 CFU, 3.90 × 10 6 CFU, 3.86 × 10 6 CFU, and 1.90 × 10 6 CFU, respectively.The concentration of bacterial solution in PBS was 2.13 × 10 5 CFU/mL, 1.95 × 10 5 CFU/mL, 1.93 × 10 5 CFU/mL, and 9.50 × 10 4 CFU/mL.The results suggest that TN-4.7-300 exhibited the best anti-bacterial adhesion response, followed by TN-0.6-300, while the performance of TN-1.9-300 was poor, and TN-1.0-300 showed a very limited resistance.Effective inhibition of bacterial adhesion may be attributed to a highly hydrophilic TiO 2 surface 14 .The dependence of WCA on pH recorded in this study is consistent with the variation in resistance to bacterial adhesion, i.e., TN-1.0-300 > TN-1.9-300 > TN-0.6-300 > TN-4.7-300.This serves to confirm that an enhancement of TiO 2 surface hydrophilicity can reduce bacterial adhesion.Bacteria spread and readily adhere to various materials and organisms, forming biofilms that are difficult to remove 57 .Therefore, it is crucial to develop highly hydrophilic surfaces that are resistant to bacterial adhesion.
Self-cleaning mechanism Drawing on the above discussion, the self-cleaning mechanism of TiO 2 is illustrated in Fig. 12.An incomplete hydrolysis of TBOT results in the generation of Ti 3+ and OVs defects, which can reduce the energy band gap in TiO 2 and enhance the response to visible light.The formation of Ti 3+ and OVs can also facilitate movement of photogenerated electrons from the valence band (VB) to the Ti 3+ /OVs energy level.This process reduces the rate of complexation of photogenerated e − -h + pairs.As a result, TiO 2 generates •O 2 -and •OH radicals when exposed to visible light, which enables the degradation of pollutants such as MO.In addition, a small TiO 2 grain size enhances surface hydrophilic properties.When a water drop contacts the surface of ahydrophilic TiO 2 film, a hydration layer is formed, which prevents adhesion of E. coli and circumvents bacterial contact infections.Ultimately, a self-cleaning TiO 2 film with photocatalytic activity and resistance to bacterial adhesion under visible light radiation is produced.

Conclusions
The crystal conformation and surface structure of anatase TiO 2 can be controlled by regulating the hydrolytic condensation and thermal crystallization processes associated with the sol-gel method, with the successful introduction of Ti 3+ and OV defects.The resultant materials exhibit good photocatalytic activity under visible light, and are hydrophilic and resistant to bacterial adhesion under natural light.Titania synthesis conditions, employing a pH of 1.0 and calcination temperature of 300 °C, yielded the most effective photodegradation catalyst under both simulated sunlight and visible light radiation.The associated first-order kinetic constants for the degradation of MO were 0.182 min −1 and 0.081 min −1 , respectively.This is attributed to the large specific surface area of TN-1.0 where the (001) crystal plane is exposed.The occurrence of Ti 3+ and OVs can reduce the band gap width of TiO 2 , which serves to enhance the photocatalytic effect under visible light.In addition, surface hydrophilicity can be controlled by adjusting the grain size.Under optimal conditions, the water contact angle of the TiO 2 film under natural light was 7.75°, less than 10°, demonstrating excellent hydrophilic properties.The amount of E. coli bacteria adhering to TiO 2 film decreased as the contact angle of the film surface decreased.This suggests that the hydrophilic TiO 2 film forms a hydrated layer that repels E. coli and prevents bacterial adhesion.

Figure 1 .
Figure 1.Process flow diagram for the preparation of TiO 2 nanopowder and thin films.

Figure 8 .
Figure 8. (a,b) Photocatalytic activities under full spectrum of as-prepared samples; (c,d) Photocatalytic activities under visible light of as-prepared samples.

Figure 12 .
Figure 12.Schematic representation of the self-cleaning mechanism for TiO 2 films.